AQUAMARINE, MAXIXE-TYPE BERYL, AND HYDROTHERMAL SYNTHETIC BLUE BERYL: ANALYSIS AND IDENTIFICATION
Ilaria Adamo, Alessandro Pavese, Loredana Prosperi, Valeria Diella, David Ajò, G. Diego Gatta, and Christopher P. Smith
Aquamarine, Maxixe-type (irradiated) beryl, and two types of hydrothermally grown synthetic blue beryl currently available in the marketplace were investigated by classical gemological methods, chemical analysis, and UV-Vis-NIR and mid-IR spectroscopy. These materials may be conclusively identified by a combination of these techniques. The Maxixe-type beryl (like natural- color Maxixe beryls) is distinguishable by its unusual dichroism, green UV fluorescence (when present), Fe-free chemical composition, and distinctive UV-Vis-NIR spectrum. The hydrothermal synthetic blue beryls can be discriminated from their natural counterparts on the basis of micro- scopic features, chemical composition, and visible and infrared spectroscopic features.
quamarine has been one of the most popular This article presents a full characterization of a gem materials for centuries, prized for its suite of aquamarines and other blue beryls of dif- A beauty and rarity. The color of aquamarine ferent origins by classic gemological and contem- ranges from the familiar light blue to blue-green porary analytical techniques, in order to determine hues, to a rarer highly saturated dark blue (e.g., those features that may be diagnostic for their Rohtert et al., 2003; Laurs, 2005). However, a deep identification. blue color is more typically associated with the color variety known as Maxixe beryl, discovered for the first time in Brazil in 1917 (Roebling and MATERIALS AND METHODS Tromnau, 1935; Schlossmacher and Klang, 1935), We examined a total of 25 natural, treated, and syn- which typically fades on exposure to light. Similar thetic blue beryl specimens (see, e.g., figure 1): four beryl specimens appeared in the market around faceted Brazilian aquamarines (0.18 to 1.54 ct); one 1973, but such material was artificially irradiated faceted and one rough aquamarine from Nigeria (1.81 and was thus called Maxixe-type beryl (Nassau et and 54.02 ct, respectively); three faceted (0.08–0.13 al., 1976). ct) and two rough (7.30 and 8.20 ct) aquamarines Synthetic blue beryl has been produced by (marketed as “True Blue” beryl) from the Yukon hydrothermal growth techniques since the late 1980s Territory, Canada; one faceted Maxixe-type (irradiat- (Koivula and Kammerling, 1988, 1991; Nassau, 1990, ed) blue beryl (1.77 ct); three faceted Tairus 1997). Tairus, a Thai/Russian joint venture, produces hydrothermal synthetic blue beryls (2.03–3.50 ct); synthetic blue beryl in Russia and markets it out of Bangkok (Smirnov et al., 1999). A new hydrothermal synthetic blue beryl was unveiled by Malossi See end of article for About the Authors and Acknowledgments. Gemme Create, Milan, Italy, during the 2006 Las GEMS & GEMOLOGY, Vol. 44, No. 3, pp. 214–226. Vegas JCK Show (A. Malossi, pers. comm., 2007). © 2008 Gemological Institute of America
214 IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 Figure 1. This study examined three vari- eties of blue beryl: aquamarine, Maxixe- type (irradiated) blue beryl, and hydrother- mally grown synthetic blue beryl. Shown here are some of those sam- ples: two aquamarines from Brazil (far left, 1.54 and 1.33 ct), one from Nigeria (bottom, 1.81 ct), one Maxixe- type beryl (center, 1.77 ct), two Tairus synthet- ics (top center, 2.03 ct and center right, 3.50 ct), and one Malossi synthetic (top right, 2.92 ct). Composite photo by Fred Kahn and Sun Joo Chung.
and eight faceted (2.70–5.12 ct) and two unfashioned Polarized ultraviolet-visible–near infrared (UV- (61.05 and 64.85 ct) Malossi hydrothermal synthetic Vis-NIR) spectroscopic measurements covering the blue beryls. 250–3300 nm range were performed with a Perkin All the faceted samples were examined by stan- Elmer Lambda 950 spectrometer using a calcite dard gemological methods to determine their opti- polarizer (1 nm scan interval) on all samples except cal properties (refractive indices, birefringence, and the Canadian and Nigerian aquamarines. pleochroism), specific gravity, UV fluorescence, and microscopic features. Quantitative chemical analyses were performed RESULTS on eight faceted samples (three aquamarines from Visual Appearance. Natural aquamarine typically Canada, one Maxixe-type beryl, and one Tairus and ranges from greenish blue to (a purer) blue of low-to- three Malossi synthetic blue beryls) using a JEOL moderate saturation with a light to medium-dark JXA-8200 electron microprobe in wavelength-dis- tone. The natural samples in this study varied in persive mode. The following elements were mea- hue, tone, and saturation (again, see figure 1). The sured: Na, Mg, Al, Si, Cl, K, Ca, Ti, V, Cr, Mn, Fe, Canadian samples were darker and more saturated Cu, Rb, and Cs. The raw data were processed for than either the Brazilian or Nigerian samples. The matrix effects using a conventional ZAF routine color of our Maxixe-type beryl was significantly from the JEOL series of programs. more intense than that typically associated with Unpolarized spectroscopic measurements over aquamarine and had a slightly violet modifier. The the near-infrared (9000–4000 cm−1) and mid-infrared Tairus and Malossi synthetic blue beryls were also (4000–400 cm−1) ranges were carried out on all but significantly more saturated and much darker in the Nigerian samples using a Nicolet Nexus Fourier- tone than most aquamarine. The Malossi samples transform infrared (FTIR) spectrometer equipped also had a distinct violet component. with a diffuse reflectance accessory (DRIFT) and operating with a resolution of 4 cm−1. Standard Gemological Properties. The standard Mid-IR spectra were also collected in transmission gemological properties of the samples included in mode using KBr pellets (2 mg sample mixed with 200 this study are summarized in table 1. mg KBr), confining the related sampling to portions of All the samples, with the exception of the Maxixe- two unfashioned specimens (one Canadian aquama- type beryl, exhibited their stronger pleochroic rine and one Malossi synthetic beryl). color perpendicular to the c-axis (e-ray). As noted by
IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 215 Figure 3. The fine, parallel growth channels in this Maxixe-type beryl indicate the natural origin of the host. Photomicrograph by Giulio Chiodi; Figure 2. Multi-phase fluid inclusions are a common magnified 50×. feature in natural aquamarine. Photomicrograph by C. P. Smith; magnified 65×.
Microscopy. The natural aquamarines and previous researchers, the stronger pleochroic color for Maxixe-type beryl in this study had a wide variety Maxixe-type beryl is observed parallel to the c-axis (o- of internal features indicative of their natural ori- ray). The Maxixe-type beryl was also the only sample gin: single- and multi-phase fluid inclusions (fig- that was not inert to both long- and short-wave UV ure 2), various patterns of healed fractures, crys- radiation. talline inclusions, and growth tubes (figure 3), as
TABLE 1. Gemological properties of the natural and synthetic blue beryls investigated in this study.
Property Aquamarine Maxixe-type Malossi Tairus (irradiated) Brazil Nigeria Canada
Color Medium blue Medium greenish Dark grayish blue Dark slightly violetish Dark violetish blue Dark grayish blue blue blue Diaphaneity Transparent Transparent Semitransparent Transparent Transparent Transparent to translucent Refractive indices no = 1.586–1.590 no = 1.586 no = 1.601 no = 1.588 no = 1.590 no = 1.586 ne = 1.580–1.582 ne = 1.578 ne = 1.592–1.593 ne = 1.580 ne = 1.582 ne = 1.580 Birefringence 0.006–0.008 0.008 0.008–0.009 0.008 0.008 0.006 Specific gravity 2.76 2.67 2.80–2.87 2.75 2.75–2.77 2.71 Pleochroisma o-ray Pale greenish blue Pale greenish blue Pale greenish blue Dark blue Pale blue Pale greenish blue e-ray Medium blue Medium blue Dark blue Colorless Dark violetish blue Dark blue UV fluorescence Long-wave Inert Inert Inert Mod. deep greenb Inert Inert Short-wave Inert Inert Inert Mod. yellowish Inert Inert green Internal features Crystals, two- Crystals, multi- Crystals, multi- Growth tubes, two- Irregular growth Irregular growth phase and liquid phase inclusions, phase inclusions, phase and liquid structures, “finger- structures, pinpoints, inclusions, “finger- growth tubes, “fingerprints,” inclusions prints,” fractures “fingerprints,” frac- prints,” growth fractures growth tubes, tures, seed plates tubes, growth lines, growth lines, frac- fractures tures, evidence of clarity enhancement a All samples were uniaxial negative, and they showed strong dichroism. b Mod. = moderate.
216 IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 Figure 4. This Malossi hydrothermal synthetic blue beryl exhibits irreg- ular growth features with a step-like shape that provide evidence of the sample’s synthetic origin. Photomicrographs by Giulio Chiodi (left, in immersion, magnified 40×) and I. Adamo (right, magnified 35×).
well as straight and angular internal growth struc- tures. Unhealed fractures were also observed in many of the aquamarine samples. However, the Canadian samples also revealed a blue and yellow “flash effect,” as is commonly observed in gems that have been clarity enhanced (refer to the “Discussion” of the mid-infrared spectroscopy results below). The Tairus and Malossi synthetic beryls also revealed several diagnostic internal features. Most notably, these consisted of distinctive irreg- ular internal growth structures (figures 4 and 5). Present in samples from both sources, but more common in those from Tairus, were healed-frac- Figure 6. “Fingerprints” (healed fractures) such as this ture “fingerprints” (figure 6), as well as open frac- one in a Tairus sample were seen in both types of syn- tures. In addition, all the Tairus synthetic sam- thetics. Photomicrograph by Giulio Chiodi, in immer- × ples contained groups of black pinpoint inclu- sion; magnified 40 . sions (figure 7), with remnants of the seed plates (in two out of the three Tairus samples; e.g., fig- ure 8) that are indicative of the artificial growth inclusions or seed-plate remnants in our Malossi process. We did not observe any of these black synthetic samples.
Figure 5. The Tairus hydrothermal synthetic samples also showed widespread irregular growth structures that demon- strate they are synthetic. Photomicrographs by I. Adamo (left, magnified 20×) and C. P. Smith (right, magnified 32×).
IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 217 Figure 7. The Tairus synthetic beryls also contained numerous small, irregular black pinpoint inclusions. Photomicrographs by C. P. Smith (left, magni- fied 32×) and Giulio Chiodi (right, in immer- sion; magnified 50×).
Chemical Composition. The chemical compositions ascribed to the presence of water in both natural and of three Canadian aquamarines, one Maxixe-type hydrothermal synthetic beryls (e.g., Wood and beryl, and one Tairus and three Malossi hydrother- Nassau, 1968; Deer et al., 1986). Totals can also be mally grown synthetic blue beryls are presented in affected by variable amounts of lithium, which— table 2 and plotted in figure 9. The low totals can be like H2O—is undetectable by electron microprobe.
TABLE 2. Average electron-microprobe analyses for the natural and synthetic blue beryls investigated in this study.a
Chemical Natural Synthetic composition Canada Maxixe-type Malossi Tairus (irradiated)
Sample 1 2 3 A B C No. analyses 5 4 5 8 10 4 4 8
SiO2 62.60 63.11 62.68 65.44 64.22 64.06 63.80 64.56 Al2O3 11.75 11.63 11.58 17.70 16.75 16.56 16.52 16.48 FeOb 5.04 5.03 4.96 bdl 1.96 1.95 2.50 2.75 MnO bdl bdl bdl bdl 0.15 0.13 0.10 bdl
K2O bdl bdl bdl 0.06 bdl bdl bdl bdl Na2O 2.24 2.40 2.24 0.47 0.07 0.12 0.13 bdl MgO 1.76 1.80 1.69 bdl 0.12 0.21 0.22 bdl
Cs2O bdl bdl bdl 0.70 bdl bdl bdl bdl CuO bdl bdl bdl bdl 2.95 1.69 1.57 bdl BeOc 12.91 12.99 12.88 13.56 12.40 12.76 12.79 13.37 Total 96.30 96.96 96.03 97.93 98.62 97.48 97.63 97.16 Ions calculated on 18 oxygens Si 6.058 6.068 6.079 6.028 6.018 6.021 6.002 6.032 Al 1.340 1.318 1.323 1.922 1.850 1.835 1.831 1.814 Fe 0.408 0.404 0.402 bdl 0.154 0.153 0.197 0.215 Mn bdl bdl bdl bdl 0.012 0.011 0.008 bdl K bdl bdl bdl 0.007 bdl bdl bdl bdl Na 0.420 0.448 0.422 0.084 0.013 0.022 0.023 bdl Mg 0.254 0.258 0.244 bdl 0.017 0.030 0.030 bdl Cs bdl bdl bdl 0.028 bdl bdl bdl bdl Cu bdl bdl bdl bdl 0.209 0.120 0.112 bdl
a Instrument operating conditions: accelerating voltage = 15 kV, beam current = 15 nA, count time = 20 seconds on peaks and 5 seconds on background. Standards: natural wollastonite (for Si, Ca), anorthite (for Al), fayalite (for Fe), olivine (for Mg), rhodonite (for Mn), omphacite (for Na), ilmenite (for Ti), K-feldspar (for K), pollucite (for Cs), and sodalite (for Cl); pure V, Rb, Cr, and Cu for those elements. Abbreviation: bdl = below detection limit (in wt.%): 0.05
FeO, 0.08 CuO, 0.04 MnO, 0.04 K2O, 0.05 Na2O, 0.05 MgO, 0.04 Cs2O. Chlorine, calcium, titanium, vanadium, chromium, and rubidium were below the detection limit (0.05 wt.%) in all analyses. b Total iron is calculated as FeO. c Calculated assuming (Be+Cu)/Si=0.5.
218 IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 Figure 8. Two of the Tairus synthetic beryls had rem- nants of the seed plate (see arrows). When present, this provides proof of synthetic origin. Note the widespread irregular growth structures, pinpoint inclusions, and “fingerprints.” Photomicrograph by Giulio Chiodi, in immersion; magnified 15×.
Consistent with the chemical formula of beryl
(Be3Al2Si6O18), all the samples contained Si, Al, and Be as major elements. Minor but significant contents of Fe, Na, and Mg were recorded in the Canadian samples, whereas Na, Cs, and traces of K were recorded in the Maxixe-type sample. The Malossi synthetic blue beryls contained high amounts of Cu
Figure 9. The average contents of Na O, MgO, MnO, 2 Figure 10. Representative mid-infrared spectra, taken FeO, CuO, and Cs2O are shown for the various types of blue beryl investigated in the present study. in diffuse reflectance, showed features between 4000 and 3400 cm−1 (and to 3200 cm−1 in the Canadian
material) related to their water contents. The CO2- related signal at 2358 cm−1 in the aquamarines and Maxixe-type beryl have thus far never been found with this strength in synthetics. The peaks between 3000 and 2800 cm−1 in the Canadian aquamarine are relat- ed to the presence of a filler (for clarity enhancement).
and Fe, as well as traces of Mg, Mn, and Na; however, Fe was the only minor element detected in the Tairus synthetic sample.
Spectroscopy. Table 3 summarizes the most signifi- cant spectroscopic features of the natural, treated, and synthetic blue beryl samples we studied, which are described below.
Mid-Infrared. The mid-infrared spectra revealed a multitude of absorption bands (figure 10). For all the samples, two dominant areas of absorption saturat- ed the detector in the 4000–3400 cm−1 (extending to 3200 cm−1 in the case of the Canadian aquamarines)
IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 219 and 2250–400 cm−1 regions. A broad band centered The presence of water in the beryl structure may between 3240 and 3220 cm−1 was also present in all be determined by careful analysis of mid-IR spectra samples. Another area of significant absorption was collected in transmission mode on powdered materi- found at approximately 2400–2250 cm−1 (again, see al in KBr pellets. This eliminates the total absorp- figure 10). In addition, we observed a series of bands tion that otherwise occurs in significant regions of in the Canadian samples in the region between that spectrum, although it does require some dam- ~3000 and 2800 cm−1 (the most dominant were at age to the original specimen. The IR pattern of a 2964, 2930, and 2872 cm−1). Malossi synthetic beryl that we acquired by this
TABLE 3. Main spectroscopic features of the natural and synthetic blue beryls investigated in this study.
Natural Synthetic Spectral region Aquamarine Malossi Tairus Brazil Canada
Mid-IR Total absorption Total absorption Total absorption Total absorption Total absorption (4000–2000 cm−1) between 4000 and between 4000 and between 4000 and between 4000 and between 4000 and 3400 cm−1, and a 3200 cm−1, with a 3400 cm−1, and a 3400 cm−1, and a 3400 cm−1, and a band at about 3240 band at 3240 cm−1, band at about 3230 band at 3230 cm−1, band at about 3220 cm−1, related to water related to water con- cm−1, related to water related to water con- cm−1, related to water content tent (in transmission content tent (in transmission content mode, resolved as mode, resolved as 3591 and 3655 cm−1 3595 and 3663 cm−1
due to type II H2O) due to type II H2O, and 3698 cm−1 due
Peaks at 3058, 3037, to type I H2O) 2964, 2930, and 2872 cm−1, due to an artificial resin
Sharp peak at about Sharp peak at 2358 Strong band at about 2358 cm−1, attributed cm−1, attributed to 2358 cm−1, attributed
to structural CO2 structural CO2 to structural CO2 Near-IR Combination bands Combination bands Combination bands Combination bands Combination bands (9000–4000 cm−1) and overtones of types and overtones of type and overtones of and overtones of and overtones of I and II water molecules II water molecules types I and II water types I and II water types I and II water molecules molecules molecules Total absorption be- tween 9000 and 6500 cm−1, likely due to the high Cu2+ content UV-Vis-NIR Strong absorption Not tested Set of bands over the Strong absorptions Strong absorption (250–850 nm) band at 825 nm (o- 500–700 nm range below 360 nm and band at 825 nm (o- and e-ray), due to Fe2+; (573, 588, 605, 625, beyond 580 nm (o- and e-ray), due to broad absorption 645, and 690 nm), re- ray) and 610 nm (e- Fe2+; broad absorption band at about 640 nm lated to a radiation- ray), due to a combi- band at about 580 nm (e-ray), assigned to a induced color center; nation of Cu and Fe (e-ray), assigned to a Fe2+↔Fe3+ charge also present were absorption features Fe2+↔Fe3+ charge process or to Fe2+ in bands at 311 nm (e-ray) process or to Fe2+ in the channels and 320 nm (o-ray) the channels Peaks at 370 nm (o- Peaks at 370 nm (o- Peaks at 370 nm (o- ray) and 427 nm (e- ray) and 428 nm (e- ray) and 428 nm (e- and o-ray), associ- and o-ray), associ- and o-ray) associ- ated with Fe3+ ated with Fe3+ ated with Fe3+ Bands at 475 and 540 nm (o-ray) and 568 nm (e-ray), probably due to Mn3+ (Ni3+ could contri- bute to the 475 nm absorption feature)
220 IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 method revealed two dominant absorption bands at 3698 and 3595 cm−1, with a weaker third band posi- tioned at ~3663 cm−1, while the Canadian aquama- rine was characterized by two dominant bands at ~3655 and 3591 cm−1 (figure 11).
Near-Infrared. As illustrated in figure 12, the signifi- cant near-infrared absorption features—strong indi- vidual bands and a number of weaker bands— occurred in the regions of ~7300–6800 cm−1 and 5650–5000 cm−1. Only the Malossi synthetic beryl exhibited total absorption beyond 6500 cm−1.
UV-Vis-NIR. Polarized UV-Vis-NIR spectra in the 280–850 nm range for four samples are shown in fig- ure 13. In general, all except the Maxixe-type blue beryl shared similar spectral features, characterized by a dominant absorption band at ~825 nm. In the spectra oriented perpendicular to the c-axis direction (e-ray), this band was modified by a side band at ~640 nm in the Brazilian aquamarine and ~580 nm in the Tairus synthetic samples. An additional band posi- tioned at 427/428 nm was evident in spectra recorded for both the e-ray and o-ray, whereas a band at 370 nm was only present in spectra oriented along the o- ray, and a weak band at ~358 nm was recorded only along the e-ray. Figure 12. Near-infrared spectra in diffuse reflectance In contrast, the absorptions recorded for the are shown for two aquamarines, a Maxixe-type beryl, Maxixe-type sample consisted of a series of narrow and Malossi and Tairus synthetic blue beryls. All except the Canadian aquamarine (which is character- ized by the absence of type I water molecules) exhibit Figure 11. Alkali-rich Canadian aquamarine and somewhat similar combination bands and overtones low-alkali Malossi synthetic beryl show different of type I and II water molecules. Note that the Malossi mid-infrared absorption spectra taken in transmis- sample exhibits total absorption between 9000 and −1 2+ sion mode on KBr pellets, because of different config- 6500 cm , most likely due to its high Cu content. urations of the water molecules hosted by the struc- tural channels. Spectra offset vertically for clarity. bands between 500 and 700 nm, with the primary band positioned at ~690 nm, and a series of associat- ed weaker bands at ~573, 588, 605, 625, and 645 nm (figure 13B). The stronger of this combined absorp- tion was oriented along the c-axis direction (o-ray). Two additional, independent bands that also exhibit- ed strongly pleochroic orientations were positioned at ~311 nm (e-ray) and 320 nm (o-ray). The Malossi synthetic blue beryl was character- ized by two strong absorptions, below about 360 nm and beyond ~580 nm (o-ray) and 610 nm (e-ray). A series of broad bands were also present, positioned at approximately 568 nm in the e-ray and at 475 and 540 nm in the o-ray orientations. The band at ~428 nm was evident in the spectra taken for both the
IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 221 Figure 13. Polarized UV-Vis-NIR spectra are shown for four samples. The aquamarine and Tairus synthetic blue beryl exhibit absorption features associated with iron, whereas the pattern of the Malossi synthetic is mainly a combination of copper and iron absorptions. Manganese may be responsible for the broad bands at 475, 540, and 568 nm in the Malossi synthetic. The spectra of the Maxixe-type beryl are characterized by signals due to radiation-induced color centers.
e- and o-ray orientations, whereas the band at 370 the Tairus synthetic specimens were similar to nm was only present along the o-ray. those reported by Schmetzer (1990) and Smirnov et al. (1999), whereas the Malossi synthetics had slight- ly higher values, owing to their compositional differ- DISCUSSION ences (notably, the presence of Cu). However, the Standard Gemological Properties. The RI and SG overlap in the ranges of RI and SG values means that values of the Brazilian and Nigerian samples were these properties cannot be used reliably to discrimi- within the ranges reported for aquamarine (RI: nate these materials from one another. 1.572–1.590; SG: 2.66–2.80; O’Donoghue, 2006). The anomalous dichroism of Maxixe-type, as well However, the Canadian samples had higher values, as Maxixe, beryls is a diagnostic marker (Brown, 1993; as previously reported by Rohtert et al. (2003). These Nassau, 1996; Reinitz and Moses, 1997; Wentzell and differences are presumably related to the chemical Reinitz, 1998). As reported by Brown (1993), the green composition (higher Fe, Mg, and Na) and denser UV fluorescence shown by the Maxixe-type sample is inclusions of the Canadian beryls. The Maxixe-type indicative of irradiation treatment. (irradiated) sample had RI and SG values that are in agreement with the literature (e.g., Brown, 1993; Microscopy. Magnification can provide important Reinitz and Moses, 1997; Wentzell and Reinitz, information for the separation of natural and syn- 1997) and are virtually identical to those of natural thetic blue beryl. Aquamarine and other natural blue Maxixe beryl (Brown, 1993). The RI and SG values of beryls may be identified by a wide range of multi-
222 IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 phase fluid inclusions; some mineral inclusions such been reported in any natural aquamarine, Maxixe- as apatite, epidote, goethite, hematite, ilmenite, type beryl, or Maxixe beryl. For information on the limonite, mica, quartz, spessartine, and tourmaline; position of Cu in the crystal structure of synthetic as well as internal growth structures (see, e.g., beryl, see Adamo et al. (2008). Sinkankas, 1981; Lindt et al., 1986; Gübelin and Tairus synthetic blue beryl may be separated Koivula, 2005). from alkali-rich natural aquamarines by its lower Fe All the synthetic blue beryls studied exhibited content and absence of any significant Cu, Na, Mg, diagnostic internal features that proved their artificial Mn, K, and Cs (see table 2 and Schmetzer et al., nature and were distinctive of hydrothermal growth. 2006). Again, though, for Na/Mg-poor natural aqua- These included strongly undulating, step- and marines such as those from Nigeria (see, e.g., Lind chevron-like growth structures, which were similar et al., 1986), chemical composition alone does not to those that have been reported for hydrothermal provide a clear distinction. synthetic emeralds (see, e.g., Schmetzer, 1988; Schmetzer et al., 1997; Sechos, 1997; Adamo et al., Spectroscopy. Mid-Infrared. All the samples revealed 2005; Gübelin and Koivula, 2005; Schmetzer et al., total absorption in the region of ~2250–400 cm−1, 2006). Residues of seed plates, when present, are also which is intrinsic to beryl, as well as ~4000–3400 diagnostic of synthetic origin. cm−1, which is related to the incorporation of water (see, e.g., Stockton, 1987; Adamo et al., 2005). Chemical Composition. Our samples could be readi- The strong 2358 cm−1 band found in natural aqua- ly separated on the basis of their chemical composi- marines and Maxixe-type beryl is attributed to struc- tion. The Canadian aquamarines had the highest tural CO2, which is commonly present in many nat- FeO contents ever reported in the literature for a ural and synthetic materials (Wood and Nassau, blue gem beryl, which were consistent with values 1967, 1968; Stockton, 1987; Aines and Rossman, reported for Canadian blue beryl by other researchers 1984; Charoy et al., 1996; Gatta et al., 2006; (Rohtert et al., 2003; Turner et al., 2007). Andersson, 2006). In beryl, however, only the natural Aquamarine specimens from other localities (e.g., material can show a strong 2358 cm−1 peak; this fea- Brazil, Mozambique, Nigeria, Arizona, and Italy) are ture is generally weak or absent in the synthetic beryl also characterized by the presence of iron (e.g., reported to date (Stockton, 1987; Koivula et al., 1996; Schaller et al., 1962; Graziani and Di Giulio, 1979; Mashkovtsev and Smirnov, 2004; Choudhary and Deer et al., 1986; Lind et al., 1986; Aurisicchio et al., Golecha, 2007). We did not observe any of the charac- 1988; Viana et al., 2002; Neiva and Neiva, 2005). Li, teristic bands attributed to chlorine and ammonium Na, Mg, K, Ca, and Cs are the most common minor that are often found in hydrothermally grown syn- elements usually present in aquamarine. Although thetic emeralds (Schmetzer et al., 1997; Mashkovtsev the distinction of natural aquamarine from alkali- and Solntsev, 2002; Mashkovtsev and Smirnov, 2004; poor synthetic beryl was straightforward for most of Adamo et al., 2005). the samples in our study, some natural stones—such The absorption features in the ~3000–2800 cm−1 as those from Nigeria (Lind et al., 1986)—have low range in the aquamarines from Canada indicate the alkali contents, so chemical composition alone presence of an organic, polymer-type filler (e.g., should not be considered proof of origin. The Johnson et al., 1999; Kiefert et al., 1999), in agree- absence of Fe, as well as of other chromophores, in ment with our microscopic observations. irradiated Maxixe-type beryl and in untreated The two dominant absorption bands at 3698 and Maxixe beryl (Schlossmacher and Klang, 1935) will 3595 cm−1 in the transmittance powder FTIR spec- easily separate them from aquamarine. trum of the Malossi synthetic blue beryl indicate the The presence of copper (CuO average 2.07 wt.%) occurrence of water molecules in two different config- is diagnostic of Malossi synthetic beryl. This well- urations [type I and type II (Wood and Nassau, 1967, known chromophore produces an intense blue col- 1968; Schmetzer and Kiefert, 1990; Charoy et al., oration in hydrothermal synthetic beryl (Koivula 1996; Mashkovtsev and Smirnov, 2004)]. The third, and Kammerling, 1988; Schmetzer et al., 2006). It is weaker and structured absorption band at approxi- also present as a trace element in some hydrother- mately 3663 cm−1 is usually also associated with type mally grown synthetic emeralds (Schmetzer, 1988; II H2O (Wood and Nassau, 1967, 1968; Farmer, 1974; Mashkovtsev and Smirnov, 2004; Adamo et al., Aines and Rossman, 1984; Charoy et al., 1996; Viana 2005; Schmetzer et al., 2006). However, it has never et al., 2002; Mashkovtsev and Smirnov, 2004),
IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 223 BOX A: IDENTIFICATION
SEPARATION BETWEEN NATURAL SEPARATION OF AQUAMARINE FROM AND SYNTHETIC BLUE BERYL MAXIXE AND MAXIXE-TYPE BERYL We found that the Malossi and Tairus synthetic blue We believe the following features provide means to beryls could be separated from their natural counter- distinguish between aquamarine and Maxixe/Maxixe- parts on the basis of the following characteristics: type beryl:
Microscopic Features. The strongly irregular and dis- Optical Properties: Dichroism. Both Maxixe and tinctive growth pattern we observed in all the synthet- Maxixe-type beryls show pleochroic behavior with the ic samples provides clear evidence of hydrothermal dominant blue color parallel to the c-axis (i.e., down synthesis. When present, the tiny black inclusions and the o-ray), which is the opposite of natural aquamarine seed-plate residues seen in the Tairus synthetic beryls and the hydrothermally grown synthetics. are also diagnostic of hydrothermal growth in a labora- tory. Natural blue beryl may be identified by a wide Other Gemological Properties. Most Maxixe/ range of multi-phase fluid inclusions, various mineral Maxixe-type beryls fade on exposure to light and/or inclusions, as well as internal growth structures. heat. A green UV fluorescence reaction, when pres- ent, provides an additional indicator that the material Chemical Composition. All aquamarines are charac- is Maxixe-type beryl. terized by the presence of iron, which acts as the pri- mary chromophore. Li, Na, Mg, K, Ca, and Cs also can Chemical Composition. The Fe chromophore is be present in variable amounts. In the case of high and absent in Maxixe and Maxixe-type beryls, but it is moderate alkali-bearing aquamarines, separation from abundant in all aquamarine from various localities. the alkali-poor Tairus synthetics is possible, but this This confirms that the cause of color in Maxixe and fails in the case of some Na/Mg-poor aquamarines, Maxixe-type beryl is a radiation-induced color center. such as Nigerian material. The presence of copper Spectroscopic Measurements. In keeping with their (average 2.07 wt.% CuO) in Malossi synthetic blue chemistry, no evidence of iron-related features occurs beryl allows a rapid distinction from natural beryl. in the UV-Vis-NIR spectra of Maxixe and Maxixe- Spectroscopic Measurements. Infrared spectroscopy type beryls. A visible spectrum with a series of bands can be diagnostic if one is able to establish the type of positioned between 500 and 700 nm will readily
water molecules: If type I H2O is absent, the beryl identify them. Color centers associated with the dif- specimen may be classified as natural; otherwise, the ferent impurities in Maxixe and Maxixe-type beryls IR pattern is not distinctive. The detection of Cu by result in slightly different UV-Vis-NIR spectra for Vis-NIR is typical of the Malossi material. these two materials.
although it may also be related to hydroxyl ions features that can be attributed to combination (Schmetzer and Kiefert, 1990; Aurisicchio et al., 1994) bands and overtones of water molecules incorporat- and/or to a third type of water molecule (Andersson, ed into the beryl structure. These spectral features 2006). Such a combination of type I and II water in are related to the presence of both type I and II beryl is typical of low-alkali-content synthetic and water molecules (Wood and Nassau, 1967; Mash- natural beryl (Schmetzer and Kiefert, 1990). In con- kovtsev and Smirnov, 2004), except for the trast, the IR spectrum of the Canadian aquamarine is Canadian aquamarine, which has no features relat- −1 distinctive in its absence of the 3698 cm absorption ed to type I H2O, as highlighted by mid-IR spec- feature (type I H2O), and it is generally diagnostic of an troscopy in transmission mode. The occurrence of alkali-rich beryl (Schmetzer and Kiefert, 1990). total absorption beyond ~6500 cm−1, attributable to the presence of Cu2+ (Mashkovtsev and Smirnov, Near-Infrared. The near-infrared spectra (9000–4000 2004; Adamo et al., 2005; Schmetzer et al., 2006), is cm−1) of all our samples revealed several absorption typical of the Malossi synthetic material.
224 IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 UV-Vis-NIR. The Brazilian aquamarines and the at about 475 nm (o-ray; Schmetzer, 1990), in agree- Tairus synthetic blue beryls revealed a typical aqua- ment with its presence among the trace elements marine spectrum, with a dominant absorption band measured by LA-ICP-MS in one Malossi sample (see positioned at ~825 nm (with polarization both paral- data in Adamo et al., 2008). lel and perpendicular to the o-ray) due to Fe2+ on two The presence in the Maxixe-type beryl of narrow different lattice positions (Wood and Nassau, 1968; absorption features in the 500–700 nm range, with the Goldman et al., 1978; Schmetzer, 1990; Burns, 1993; dominant band at ~690 nm, as well as the vibronic Taran and Rossman, 2001; Viana et al., 2002). A side structure that extends toward 400 nm, has been band positioned at ~640 nm in the natural aquama- attributed to color centers associated with carbonate rine and ~580 nm in the Tairus synthetic material impurities that have been activated by irradiation (with polarization perpendicular to the o-ray) is also (Nassau et al., 1976; Edgar and Vance, 1977; present. This absorption feature has been assigned by Andersson, 1979; Nassau and Prescott, 1981; Nassau, some to an Fe2+↔Fe3+ charge-transfer process (e.g., 1996; Mathew et al., 1998; Andersson, 2006). In the Goldman et al., 1978; Schmetzer, 1990; Burns, 1993; original Maxixe beryl, these color centers are associat- Taran and Rossman, 2001), whereas others (e.g., ed instead with nitrate impurities, causing a slightly Wood and Nassau, 1968; Viana et al., 2002) have sug- different visible spectrum (Andersson, 1979, Nassau, gested that it arises from Fe2+ in the structural chan- 1996). Thus, the UV-Vis-NIR spectra for both Maxixe nels. The peaks at 370 and 428 nm are related to Fe3+ and Maxixe-type beryls provide reliable means to dis- (Goldman et al., 1978; Schmetzer, 1990; Burns, 1993; tinguish these gem materials from aquamarine. Viana et al., 2002; Adamo et al., 2005). Distinctive of the Malossi synthetic blue beryl was a very strong absorption (even more intense than CONCLUSIONS in other samples) starting at ~610 nm (e-ray) and 580 Aquamarine, Maxixe-type beryl, and hydrother- nm (o-ray) and extending to 1500 nm in the near-IR mally grown synthetic blue beryl may be readily region, which may result from a combination of cop- distinguished using a combination of gemological, per and iron absorptions (see, e.g., Mashkovtsev and chemical, and spectroscopic features (see box A). Smirnov, 2004; Adamo et al., 2005; Schmetzer et al., Careful observation of pleochroism, fluorescence, 2006). The 370 and 428 nm Fe3+ absorption features and internal features (with magnification) can pro- were also present. The broad bands centered at 475, vide useful indicators for gemologists with basic 540, and 568 nm are probably related to Mn3+, a chro- equipment. More-sophisticated techniques such as mophore known to produce pink, red, and violet UV-Vis-NIR and mid-infrared spectroscopy, as hues in beryl (Burns, 1993; Shigley et al., 2001). Ni3+ well as chemical analysis, can provide clear proof might also contribute to the broad absorption feature of the identification.
ABOUT THE AUTHORS Brazil, the Maxixe-type blue beryl specimen, and the Tairus Dr. Adamo ([email protected]) is a postdoctoral fellow, Dr. hydrothermal synthetic blue beryls; Alberto Malossi (Malossi Pavese is professor of mineralogy, and Dr. Gatta is a researcher Gemme Create, Milan) for providing the Malossi synthetic blue in the Earth Sciences Department of the University of Milan, Italy. beryl samples; and C. R. “Cap” Beesley (AGL) for providing the Dr. Prosperi is director of the Italian Gemological Institute (IGI) aquamarine samples from Brazil and Nigeria. Dr. Giulio Chiodi laboratory, Milan. Dr. Diella is a senior researcher of the (Vicenza, Italy), Fred Kahn, and Sun Joo Chung (AGL) are grate- Environmental Processes Dynamics Institute (IDPA), National fully acknowledged for some photos. The authors are indebted Research Council (CNR), Section of Milan, to which Dr. Pavese for technical assistance to: Dr. Vanda Rolandi (University of and Dr. Gatta also belong. Dr. Ajò is director of the Inorganic and Milan—Bicocca, Italy) and Stefano Villa (IGI, Milan) for collabora- Surface Chemistry Institute (ICIS), National Research Council tion in the collection of photomicrographs; Dr. Marcello Picollo, (CNR), Padua, Italy, and is responsible for the CNR coordination Bruno Radicati (CNR, Florence), and Franco De Zuane (CNR, group for Gemological Materials Research. Mr. Smith is vice Padua) for preliminary nonpolarized UV-Vis-NIR spectroscopy; president and chief gemologist at American Gemological and Dr. Nicola Rotiroti (University of Milan) for collaboration in X- Laboratories (AGL) in New York City. ray single-crystal data collection and structure refinement. Dr. Karl Schmetzer (Petershausen, Germany) is thanked for his use- ACKNOWLEDGMENTS ful suggestions. The manuscript benefited considerably from the The authors would like to thank Greg Davison (True North Gems, critical reviews of Dr. Lee A. Groat and Dr. Michael S. Vancouver, Canada) for providing the blue beryl specimens from Krzemnicki. This study was supported through the Ingenio the True Blue property in the Yukon Territory, Canada; the Italian Global Grant project by the European Social Fund, the Italian Gemological Institute for providing aquamarine samples from Ministry of Labour and Welfare, and the Lombardy Region.
IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008 225 REFERENCES pp. 65–71. Adamo I., Gatta G.D., Rotiroti N., Diella V., Pavese A. (2008) Mathew G., Karanthy R.V., Gundu Rao T.K., Deshpande R.S. (1998) Gemmological investigation of a synthetic blue beryl: A multi- Maxixe-type colour centre in natural colourless beryl from Orissa, methodological study. Mineralogical Magazine (in press). India: An ESR and OA investigation. Journal of Gemmology, Vol. 26, Adamo I., Pavese A., Prosperi L., Diella V., Merlini M., Gemmi M., Ajò D. No. 4, pp. 238–251. (2005) Characterization of the new Malossi hydrothermal synthetic Nassau K. (1990) Synthetic gem materials in the 1980s. Gems & emerald. Gems & Gemology, Vol. 41, No. 4, pp. 328–338. Gemology, Vol. 26, No. 1, pp. 50–63. Aines R.D., Rossman G.R. (1984) The high temperature behavior of water Nassau K. (1996) On the identification and fade testing of Maxixe beryl, and carbon dioxide in cordierite and beryl. American Mineralogist, golden beryl and green aquamarine. Journal of Gemmology, Vol. 25, Vol. 69, No. 3/4, pp. 319–327. No. 2, pp. 108–115. Andersson L.O. (1979) The difference between Maxixe beryl and Maxixe- Nassau K. (1997) The chronology of synthetic gemstones. Journal of type beryl: An electron paramagnetic resonance investigation. Journal Gemmology, Vol. 25, No. 7, pp. 453–516. of Gemmology, Vol. 16, No. 5, pp. 313–317. Nassau K., Prescott B.E. (1981) Nonfading Maxixe-type beryl? Gems & Andersson L.O. (2006) The position of H+, Li+ and Na+ impurities in beryl. Gemology, Vol. 17, No. 4, pp. 217–219. Physics and Chemistry of Minerals, Vol. 33, No. 6, pp. 403–416. Nassau K., Prescott B.E., Wood D.L. (1976) The deep blue Maxixe-type color Aurisicchio C., Fioravanti G., Grubessi O., Zanazzi P.F. (1988) Reappraisal center in beryl. American Mineralogist, Vol. 61, No. 1/2, pp. 100–107. of the crystal chemistry of beryl. American Mineralogist, Vol. 73, No. Neiva A.M.R., Neiva M.C.J. (2005) Beryl from the granitic pegmatite at 7/8, pp. 826–837. Nativo, Alto Ligonha, Mozambique. Neues Jahrbuch für Mineralogie, Aurisicchio C., Grubessi O., Zecchini P. (1994) Infrared spectroscopy and Abhandlungen, Vol. 181, No. 2, pp. 173–182. crystal chemistry of the beryl group. Canadian Mineralogist, Vol. 32, O’Donoghue M. (2006) Gems, 6th ed. Butterworth-Heinemann, Oxford, UK. No. 1, pp. 55–68. Reinitz I., Moses T. (1997) Lab Notes: Beryl, treated color. Gems & Brown G. (1993) Maxixe-type beryls. Ghost from the past. Australian Gemology, Vol. 33, No. 4, p. 293. Gemmologist, Vol. 18, No. 7, pp. 215–221. Roebling W., Tromnau H.W. (1935) Maxixeberyll. II. Zentralblatt für Burns R.G. (1993) Mineralogical Applications of Crystal Field Theory, 2nd Mineralogie, Geologie und Paläontologie, Vol. A, pp. 134–139. ed. Cambridge Topics in Mineral Physics and Chemistry, Cambridge Rohtert W.R., Quinn E.P., Groat L.A., Rossman G.R. (2003) Gem News University Press, Cambridge, UK. International: Blue beryl discovery in Canada. Gems & Gemology, Charoy B., De Donato P., Barres O., Pinto-Coelho C. (1996) Channel occu- Vol. 39, No. 4, pp. 327–329. pancy in an alkali-poor beryl from Serra Branca (Goiás, Brazil): Schaller W.T., Stevens R.E., Jahns R.H. (1962) An unusual beryl from Spectroscopic characterization. American Mineralogist, Vol. 81, No. 3/4, Arizona. American Mineralogist, Vol. 47, No. 5/6, pp. 672–699. pp. 395–403. Schlossmacher K., Klang H. (1935) Der Maxixeberyll. I. Zentralblatt für Choudhary G., Golecha C. (2007) Gem News International: New Tairus Mineralogie, Geologie und Paläontologie, Vol. A, pp. 37–44. synthetic beryl simulating “Paraíba” tourmaline. Gems & Gemology, Schmetzer K. (1988) Characterization of Russian hydrothermally grown Vol. 43, No. 4, pp. 385–387. synthetic emeralds. Journal of Gemmology, Vol. 21, No. 3, pp. 145–164. Deer W.A., Howie R.A., Zussman J. (1986) Disilicates and Ring Silicates. Schmetzer K. (1990) Hydrothermally grown synthetic aquamarine manu- Rock-Forming Minerals, Vol. 1B, Geological Society of London, UK, factured in Novosibirsk, USSR. Gems & Gemology, Vol. 26, No. 3, pp. pp. 373–409. 206–211. Edgar A., Vance E.R. (1977) Electron paramagnetic resonance, optical Schmetzer K., Kiefert L. (1990) Water in beryl—A contribution to the sepa- - absorption, and magnetic circular dichroism studies of the CO3 molec- rability of natural and synthetic emeralds by infrared spectroscopy. ular-ion in irradiated natural beryl. Physics and Chemistry of Journal of Gemmology, Vol. 22, No. 4, pp. 215–223. Minerals, Vol. 1, No. 2, pp. 165–178. Schmetzer K., Kiefert L., Bernhardt H-J., Beili Z. (1997) Characterization of Farmer V.C. (1974) The Infrared Spectra of Minerals. Mineralogical Chinese hydrothermal synthetic emerald. Gems & Gemology, Vol. 33, Society, London. No.4, pp. 276–291. Gatta G.D., Nestola F., Bromiley G.D., Mattauch S. (2006) The real topo- Schmetzer K., Schwarz D., Bernhardt H-J, Häger T. (2006) A new type of logical configuration of the extra-framework content in alkali-poor Tairus hydrothermally-grown synthetic emerald, coloured by vanadi- beryl: A multi-methodological study. American Mineralogist, Vol. 91, um and copper. Journal of Gemmology, Vol. 30, No. 1/2, pp. 59–74. No. 1, pp. 29–34. Sechos B. (1997) Identifying characteristics of hydrothermal synthetics. Goldman D.S., Rossman G.R., Parkin K.M. (1978) Channel constituents in Australian Gemmologist, Vol. 19, No. 9, pp. 383–388. beryl. Physics and Chemistry of Minerals, Vol. 3, No. 3, pp. 225–235. Shigley J.E., McClure S.F., Cole J.E., Koivula J.I., Lu T., Elen S., Demianets Graziani G., Di Giulio V. (1979) Growth of aquamarine crystal from Brazil. L.N. (2001) Hydrothermal synthetic red beryl from the Institute of Neues Jahrbuch für Mineralogie—Monatshefte, Vol. 3, pp. 101–108. Crystallography, Moscow. Gems & Gemology, Vol. 37, No. 1, pp. Gübelin E.J., Koivula J.I. (2005) Photoatlas of Inclusions in Gemstones, 42–55. Vol. 2. Opinio Publishers, Basel, Switzerland. Sinkankas J. (1981) Emerald and Other Beryls. Chilton Book Co., Radnor, Johnson M.L., Elen S., Muhlmeister S. (1999) On the identification of var- PA. ious emerald filling substances. Gems & Gemology, Vol. 35, No. 2, Smirnov S., Mashkovtsev R., Thomas V., Maltsev V., Alexey I., Anastasiya pp. 82–107. B. (1999) New hydrothermal synthetic gemstones from Tairus, Kiefert L., Hänni H.A., Chalain J-P., Weber W. (1999) Identification of filler Novosibirsk, Russia. Gems & Gemology, Vol. 35, No. 3, pp. 175–176. substances in emeralds by infrared and Raman spectroscopy. Journal of Stockton C.M. (1987) The separation of natural from synthetic emerald. Gemmology, Vol. 26, No. 8, pp. 501–520. Gems & Gemology, Vol. 23, No. 2, pp. 96–99. Koivula J.I., Kammerling R.C. (1988) Gem News: Unusual synthetic beryls Taran M.N., Rossman G.R. (2001) Optical spectroscopy study of tuhualite from the Soviet Union. Gems & Gemology, Vol. 24, No. 4, pp. 252–253. and a re-examination of the beryl, cordierite, and osumilite spectra. Koivula J.I., Kammerling R.C. (1991) Gem News: More Soviet synthetics. American Mineralogist, Vol. 86, No. 9, pp. 973–980. Gems & Gemology, Vol. 27, No. 1, pp. 55. Turner D., Groat L.A., Hart C.J.R., Mortensen J.K., Linnen R.L., Giuliani Koivula J.I., Kammerling R.C., DeGhionno D., Reinitz I., Fritsch E., G., Wengzynowski W. (2007) Mineralogical and geochemical study of Johnson M.L. (1996) Gemological investigation of a new type of the True blue aquamarine showing, southern Yukon. Canadian Russian hydrothermal synthetic emerald. Gems & Gemology, Vol. 32, Mineralogist, Vol. 45, No. 2, pp. 203–227. No. 1, pp. 32–39. Viana R.R., Jordt-Evangelista H., Magela da Costa G., Stern W.B. (2002) Laurs B.M. (2005) Gem News International: Saturated blue aquamarine Characterization of beryl (aquamarine variety) from pegmatites of from Nigeria. Gems & Gemology, Vol. 41, No. 1, p. 56. Minas Gerais, Brazil. Physics and Chemistry of Minerals, Vol. 29, No. Lind T., Schmetzer K., Bank H. (1986) Blue and green beryls (aquamarines 10, pp. 668–679. and emeralds) of gem quality from Nigeria. Journal of Gemmology, Wentzell C.Y., Reinitz I. (1998) Lab Notes: Maxixe beryl, faded and fading. Vol. 20, No. 1, pp. 40–48. Gems & Gemology, Vol. 34, No. 4, pp. 284–285. Mashkovtsev R.I., Smirnov S.Z. (2004) The nature of channel constituents Wood D.L., Nassau K. (1967) Infrared spectra of foreign molecules in beryl. in hydrothermal synthetic emerald. Journal of Gemmology, Vol. 29, Journal of Chemical Physics, Vol. 47, No. 7, pp. 2220–2228. No. 3, pp. 129–141. Wood D.L., Nassau K. (1968) The characterization of beryl and emerald by Mashkovtsev R.I., Solntsev V.P. (2002) Channel constituents in synthetic visible and infrared absorption spectroscopy. American Mineralogist, beryl: Ammonium. Physics and Chemistry of Minerals, Vol. 29, No. 1, Vol. 53, No. 5/6, pp. 777–800.
226 IDENTIFICATION OF NATURAL AND SYNTHETIC BLUE BERYL GEMS & GEMOLOGY FALL 2008